# Ab initio study of structural, electronic and ... · 3.2. Electronic properties All electronic...

Embed Size (px)

### Transcript of Ab initio study of structural, electronic and ... · 3.2. Electronic properties All electronic...

Ab initio study of structural, electronic and thermodynamic propertiesof tungstate double perovskites Ba2MWO6 (M = Mg, Ni, Zn)

O. Sahnoun a,c,⇑, H. Bouhani-Benziane a, M. Sahnoun a, M. Driz b, C. Daul c

a Laboratoire de Physique Quantique de la Matière et Modélisation Mathématique (LPQ3M), University of Mascara, Algeriab Laboratoire de Sciences des Matériaux (LSM), University of Sidi Bel Abbes, AlgeriacDepartment of Chemistry, University of Fribourg, Switzerland

The structural and electronic properties of the double perovskite Ba2MWO6 with M = Mg, Ni, Zn havebeen studied using the full-potential linearized augmented plane wave (FP-LAPW) method by employingboth the local density approximation (LDA) and the generalized gradient approximation (GGA), which arebased on exchange–correlation energy optimization to calculate the total energy. Also we have used theEngel–Vosko GGA formalism, which optimizes the corresponding potential for band structure calcula-tions. However, we have evaluated the ground state quantities such as lattice parameter, bulk modulusand its pressure derivative. Also, we have presented the results of the band structures and densities ofstates. These results were in favorable agreement with previous theoretical works and the existing exper-imental data. To complete the fundamental characteristics of these compounds we have analyzed thethermodynamic properties such as thermal expansion coefficient, heat capacities and other structuralparameters in the whole pressure range from 0 to 20 GPa and temperature range from 0 to 1000 K.

1. Introduction

Because of their variable structure and composition, perovskitematerials have attracted intense research interest in many appliedand fundamental areas of solid-state science and advanced materi-als research at least for half a century. The perovskite structure(with general formula ABO3) can be described as a framework ofoxygen octahedral sharing corners [1,2]. The B-cations are locatedin the centers of octahedra and the interstitial sites are occupied bythe A-cations. In complex perovskites two (or more) cations of dif-ferent valences are located in the equivalent crystallographic posi-tions [3]. Among the A2B0B0 0O6 complex perovskite oxides, where B0

and B0 0 are the cations of different valences, the mixed alkalineearth tungstate double perovskites with the general formulaA2BWO6 (A = Ba, Sr, Ca; B = Mg, Co, Zn, Ni) are of interest for theircomplete 1:1 ordered state due to their larger differences in chargeand ionic radii on B-site [4]. The barium containing tungstate dou-ble perovskites were determined to be cubic and in the space groupFm3m [5]. Ba2MWO6 (where M = Ni, Mg) have shown great poten-tial as ceramic components for temperature sensors for example inpetroleum wells [6]. These ceramics were produced by solid-statereaction process and sintered at different sintering conditions [7].Understanding properties of these compounds and related materi-

als at the atomistic level may help to improve the performance oftheir applications. Despite the recent progress in understandingthe physics of the double perovskites there is still an open debateon the adequate theoretical modeling. In particular, the details ofthe interplay between structural, electronic, and magnetic degreesof freedom in the double perovskites are not yet clearly under-stood. To our knowledge, there is less or none theoretical studiesin the literature devoted to electronic and thermal properties ofmixed alkaline earth tungstate double perovskites.

The aim of this work is to provide information of some orderedtungstate double perovskites, and describes results for three ofthese, namely Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6. These partic-ular compounds are reported to be cubic at room temperature [8],in contrast to many others which are somewhat distorted. The pa-per is organized as follows: in Section 2 we briefly describe thetechnical details of the employed methods for calculations. Sec-tion 3 presents and discusses the results of the electronic and ther-modynamic properties. A summary concludes the paper inSection 4.

2. Computational details

The calculations presented in this work were performed usingthe FP-LAPWmethod, as implemented in the Wien2k code [9]. Thismethod allows the inclusion of local orbital in the basis, improvingupon linearization and making possible a consistent treatment of

⇑ Corresponding author at: Laboratoire de Physique Quantique de la matière etModélisation Mathématique (LPQ3M). University of Mascara, Algeria.

E-mail address: [email protected] (O. Sahnoun).

1

Published in "which should be cited to refer to this work.

http

://do

c.re

ro.c

h

semicore and valance states in an energy window, hence ensuringproper orthogonality. It is well known in the self-consistent bandstructure calculation within DFT [10], both LDA [11] and general-ized gradient approximation (GGA) [12] usually underestimatesthe energy gap [13]. This is mainly due to the fact that they havesimple forms that are not sufficiently flexible to accurately repro-duce both the exchange–correlation energy and its charge deriva-tive. Engel and Vosko considered this shortcoming and constructeda new functional form of GGA [14] which is able to better repro-duce the exchange potential at the expense of less agreement inthe exchange energy. This approach called EV-GGA yields betterband splitting and some other properties which mainly dependon the accuracy of exchange–correlation potential.

All the calculations were converged with respect to Brillouinzone (BZ) sampling and the size of the basis set. Brillouin zone(BZ) integrations within the self-consistency cycles were per-formed via a tetrahedron method, using 8 � 8 � 8 special k-pointsmesh [15]. The convergence parameter RmtKmax, which controls thesize of the basis sets, was set to 8. The Gmax parameter was taken tobe 12 Bohr�1. The muffin-tin radii were taken as (2.5, 1.8, 1.6, 2.0,2.0, 1.98) a.u. for (Ba, W, O, Mg, Ni, Zn), respectively. Careful con-vergence tests show that with these parameters relative energyconverged to better than 10�5 Ry per formula unit.

3. Results and discussion

3.1. Structural properties

We employed the experimentally observed cubic crystallinestructures [16] for the three compounds in the calculation, whichcan be described by the space group Fm3m, with Ba ions in 8(c)positions at 1/4, 1/4, 1/4; M (M = Mg, Ni or Zn) in 4(a) at 0,0,0;W in 4(b) at 1/2, 1/2, 1/2; and O in 24(e) at x,0,O. In the orderedcubic double perovskites Ba2MWO6 (M = Mg, Ni or Zn), the Mand W cations are octahedrally coordinated by oxygen anions(see Fig. 1). In this aristotype cubic structure, the highly electropos-itive Ba cation is coordinated to 12 oxygens, while each M cationhas 6 W cations as nearest neighbors and vice versa. With thisarrangement the intermediate oxygen anions can satisfy the differ-ent bond length requirements of the two cations by moving towardthe smaller ion. This structure is often viewed in terms of an or-dered alternation of M and W cation layers perpendicular to the[111] direction. The lattice parameters, the bulk moduli and theoxygen parameter x which can deviate from the ideal value of0.25 realized in the simple perovskite structure, are summarized

in Table 1, together with the available experimental [17–21] andother theoretical calculation data [22–26]. It can be seen that cal-culated lattice constants are overestimated with the experimentaldata not more than 1%, which indicates that the present calcula-tions are highly reliable. In the current work, the bulk modulus isin reasonable agreement with other theoretical calculations inthe case of Ba2MgWO6.

3.2. Electronic properties

All electronic properties have been calculated for the equilib-rium geometry. We collected data on the optical gaps in Table 2.In Fig. 2 we presented the band structures for each crystal calcu-lated using the Engel–Vosko GGA formalism. It can be seen fromFig. 2 that the conduction band (CB) structure is nearly unaffectedby the different B-cations in the lattice while the top of valenceband (VB) increases inducing an obvious band gap narrowing.The bottom of the conduction band lies at the X-point in all threedouble-perovskite crystals. The electron energy in the lowest con-duction band at the X-point is just 0.7–1.3 eV higher than at thebottom of conduction bands. So, there is a little dispersion in thelowest conduction band between the W, L and X points in the Brill-ouin zone. The top of the valence band is displaced from the L pointof the Brillouin zone in Ba2NiWO6 and Ba2ZnWO6 to the C-point inBa2MgWO6. The highest valence electron states at the C-point ap-pear only about 0.05 eV below the highest states in X-point forboth Ba2MgWO6 and Ba2ZnWO6 compounds. The dispersion ofthe top valence band is almost flat between C and X points forthese two compounds. The additional d-orbitals on Zn ions in Ba2-ZnWO6 cause the appearance of an additional valence band belowthe other bands. They cause also the highest states at the C-pointto rise above all other valence states and to make a new top of thevalence band. The effect of the electronic structure perturbationcaused by different B-cations located in the centers of octahedrais illustrated by a comparison of the total and projected densitiesof states (DOSs) for the three compounds Ba2MgWO6, Ba2NiWO6

and Ba2ZnWO6. From Fig. 3, we can find that the DOS can be mainlydivided into four parts. The first part extending from �11 to�9.5 eV is characterized by a peak mainly due to the contributionof Ba ions. On the other hand, near the Fermi level (EF) until

Fig. 1. The crystal structure of double perovskite Ba2MWO6.

Table 1Summary of calculated lattice constants (Å), the oxygen parameter x, and bulkmodulus (GPa) of Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6 at zero pressure, comparedwith experimental and other theoretical data.

a (Å) B (GPa) B0 x

Ba2MgWO6

LDA 8.016 187.78 4.44 0.259GGA 8.095 175.87 4.65 0.261Exp. [17] 8.1345 137.00 3.90 0.241Exp. [18] 8.112Exp. [19] 8.1046Cal. [22] 8.099Cal. [23] 8.0166 149.67 4.51 0.239

Ba2NiWO6

LDA 7.943 201.86 4.69 0.258GGA 8.032 187.22 4.70 0.259Exp. [20] 8.060 0.260Exp. [21] 8.066Cal. [24] 8.064

Ba2ZnWO6

LDA 8.023 193.78 4.70 0.261GGA 8.110 180.15 4.50 0.262Exp. [19] 8.1362Exp. [21] 8.1216Cal. [24] 8.137Cal. [25] 0.236Cal. [26] 0.237

2

http

://do

c.re

ro.c

h

�5.7 eV for Ba2(Mg,Zn)WO6 and �7 eV for Ba2NiWO6, consists pre-dominantly of oxygen (O) ion, but contains a small admixture ofMg, Ni, and Zn and W ions. The oxygen p-orbitals give the primarycontribution to the valence band of all three studied perovskites.These O 2p-orbitals are perpendicular to the W–O–M (M = Mg,Ni, Zn) bridge and lie in the BaO-planes. The additional valencebands contain contributions mostly from W 6s-orbitals. Theseorbitals contribute to the valence bands through the entire set ofthe bands. In the conduction band both the oxygen (O) and tung-sten (W) ions contribute to roughly the same amount, which isextending from 3.10 to 4.30 eV for Ba2(Mg,Zn)WO6 and 2.30 to3.20 eV for Ba2NiWO6. Last part, at higher energies of the conduc-tion band, consists of Ba, Mg, W, and O ions, but a small from Ni,Zn. From Fig. 3, it can be found that the PDOS of Ba and W atomshave almost the same contribution to DOS for the three com-pounds Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6. Many of the W 5dstates are empty and located above EF, while also a few states oc-cupy the region below EF due to the strong hybridization with oxy-gen. The optical band gaps of the three double-perovskitesobtained using different functionals are summarized in Table 2.This table clearly demonstrates that both LDA and GGA calcula-tions dramatically underestimate the optical gap by several timesfor all three perovskites. This tendency is well known in solid statephysics [27]. The most realistic band gaps have been obtainedusing the Engel–Vosko GGA functional, in agreement with avail-

Table 2Summary of calculated band gaps (eV) compared with experimental and othertheoretical data.

Band gap EV-GGA LDA GGA Exp. Cal.

Ba2MgWO6

C–C 3.316 2.515 2.450X–X 3.056 2.412 2.303W–W 4.017 3.214 3.265L–L 4.038 3.204 3.289L–X 3.400 2.706 2.749C–X 3.000 2.349 2.303 3.4 [28] 2.89 [28,23]

3.5 [29]

Ba2NiWO6

C–C 3.609 2.833 3.019X–X 2.970 2.350 2.528W–W 3.048 2.041 2.283L–L 2.450 1.520 1.758L–X 2.204 2.870 1.562C–X 3.265 2.586 2.823

Ba2ZnWO6

C–C 3.633 2.589 3.658X–X 3.404 2.588 3.300W–W 4.173 3.126 4.130L–L 3.530 2.476 3.457L–X 3.064 2.144 3.000 3.5 [28]

3.8 [29]C–X 3.314 2.423 3.274

Fig. 2. Calculated band structures of (a) Ba2MgWO6, (b) Ba2NiWO6 and (c) Ba2ZnWO6.

Fig. 3. Calculated partial density of states and total density of states of (a) Ba2MgWO6, (b) Ba2NiWO6 and (c) Ba2ZnWO6.

3

http

://do

c.re

ro.c

h

able studies. The Ba2MgWO6 experimental band gap is 3.4 eV (indi-rect gap), as determined by Eng et al. using the UV–visible diffusereflectance spectroscopy [28], 3.5 eV band gap has also been mea-sured for Ba2ZnWO6 [29]. In our calculations using the Engel–Vos-ko GGA functional, we have obtained the Ba2MgWO6 indirect bandgap (C–X) of 3.06 eV. The value of 2.20 eV has been obtained forthe indirect band gap (L–X) of Ba2NiWO6 and the value of3.068 eV for the Ba2ZnWO6 indirect band gap (L–X). Our band gapsare in a good agreement with the experiment, the discrepancy isless than 10%. This is acceptable if we take into account difficultiesin determining experimentally the band gap, including the opticalabsorption edge tails which extend up to several tenths of eV.

3.3. Thermodynamic properties

The thermal properties are determined by using a quasi-harmonic Debye, in which the non-equilibrium Gibbs functionG�(V; P, T) is written in the form:

G�ðV ; P; TÞ ¼ EðVÞ þ PV þ Fvib½HðVÞ; T� ð1Þwhere E(V) is the total energy per unit cell, PV corresponds to theconstant hydrostatic pressure condition, H(V) is the Debye temper-ature and Avib is the vibrational term which can be written using theDebye model of the phonon density of states as:

Fvib½HðVÞ; T� ¼ NkBT9H8T

þ 3 ln 1� e�HT

� �� D

HT

� �� �ð2Þ

where D(H/T) represents the Debye integral, N the number of atomsin a chemical formula. Using a quasi-harmonic Debye model in theSlater formulation, the Debye temperatures HD(V) are computedfrom the static bulk moduli BS(V), and the Poisson ratio is assumedto be volume independent, and equal to 1/4, corresponding to aCauchy solid. This method, implemented in the GIBBS code and de-scribed with detail in Ref. [30], requires only a collection of {V, E(V)}points around the equilibrium geometry. Assuming isotropic condi-tions, with Poisson ratio m, HD can be given by [30,31]:

HD ¼ hkB

6p2V1=2Nh i1=3

f ðmÞffiffiffiffiffiBS

M

rð3Þ

where M is the molecular mass per formula unit, and f(m) is givenby:

f ðmÞ ¼ 3 223

1þ m1� 2m

� �3=2

þ 131þ m1� m

� �3=2" #�1

8<:

9=;

1=3

ð4Þ

The static bulk modulus is given by the curvature of the E(V)function:

BS ffi Bstatic ¼ Vd2EðVÞdV2

!ð5Þ

The curvature of the E(V) function changes with the volume,increasing sharply as the crystal volume decreases, and decreasingin a lesser amount as the crystal expands. This asymmetry betweenthe curvature at the left and at the right of the equilibrium volumeis the origin of the volume dependence of HD and it is the mainreason behind the capability of the quasi-harmonic Debye modelto predict the low temperature behavior of the crystal, includingthe V(T) dependency. Accordingly, the non-equilibrium Gibbs func-tion G�(V; P, T) as a function of V, P and T can be minimized withrespect to volume V:

@G�ðV ; P; TÞ@V

� �P;T

¼ 0 ð6Þ

By solving Eq. (6), one can obtain the thermal equation-of-state(EOS) V(P, T). The heat capacity at constant volume CV, the thermalexpansion coefficient a, and the heat capacity at constant pressureCP, are given respectively by [30]:

CV ¼ CV ðVðp; TÞ; TÞ ¼ @G�

@T

� �V¼ 3NkB 4D

HT

� �� 3H=TeH=T � 1

� �ð7Þ

a ¼ cCV

BTVð8Þ

BT is the isothermal bulk modulus given by:

BT ¼ �[email protected]@V

� �T¼ V

!T

ð9Þ

CP ¼ CV ð1þ caTÞ ð10Þwhere c is the Grüneisen parameter which is approximated as [32]:

c ¼ � d lnðHðVÞÞd lnV

ð11Þ

Fig. 4. The relationship between (a) lattice constants and (b) bulk modulus with pressure at temperatures of 0 K, 400 K, 800 K, and 1000 K, respectively.

4

http

://do

c.re

ro.c

h

c is calculated using a fit to entropy values at very low but not zerotemperatures, for any volume. The thermal properties are deter-mined in the temperature range from 0 to 1000 K, where the qua-si-harmonic model remains fully valid. The pressure effect isstudied in the 0–20 GPa range. The temperature effects on the lat-tice parameters are shown in Fig. 4. The lattice parameter increaseswith increasing temperature but the rate of increase is very moder-ate. It is also noted from the regular spacing of the curves in Fig. 4that the relationships between bulk modulus and pressure are allnearly linear at various temperatures of 0, 200, 400, 600, 800 and1000 K, respectively. The bulk modulus increases with pressure ata given temperature. However, the effect of increasing pressureon the material is the same as decreasing temperature of thematerial.

The calculated heat capacity at constant pressure CP and heatcapacity at constant volume CV with the temperature T at differentpressure P are shown in Fig. 5. The changing trends of the heat

capacity of the three double-perovskite structures are similar.The difference between CP and CV is very small at low tempera-tures. However, at high temperatures, the CV approaches a constantvalue, CP increases monotonously with increments of the tempera-ture. The values follow the Debye model at low temperature(CV(T) / T3), this is because only the long wavelength vibrationmodes of the lattice are populated and these modes could beapproximated by treating the lattice as a continuum. However,the classical behavior (CV(T) / 3R for mono-atomic solids) is foundat sufficient high temperatures, which is in agreement with the lawof Petit and Dulong [33]. From Fig. 5, one can also see that the heatcapacity increases with the temperature at the same pressure anddecreases with the pressure at the same temperature, the influ-ences of the temperature on the heat capacity are much moresignificant than that of the pressure on it.

The Debye temperature is the key quantity in the quasi-harmonic Debye model, which correlates with many physical

Fig. 5. Pressure and temperature dependence of (a) Debye temperature and (b) thermal expansion coefficient of Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6.

Fig. 6. Temperature dependence of (a) constant pressure heat capacity (Cp) and (b) constant volume heat capacity (Cv) of Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6.

5

http

://do

c.re

ro.c

h

properties of solids, such as specific heat, elastic constants andmelting temperature. We calculate dependence of the Debye tem-perature on pressure and temperature as shown in Fig. 6. The cal-culated value of Debye temperature at 0 K and 0 GPa is 512.58 K,510.20 K, 515.20 K, for Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6,respectively. When the external pressure changes from 0 to20 GPa, the calculated Debye temperature increases by (18.32%,18.57%, 19.20%) and (26.13%, 26.60%, 27.48%) at temperatures of0 and 1000 K, for all the three compounds, respectively. Addition-ally, it is seen in Fig. 6 that the Debye temperature decreases withtemperature at a constant pressure and at a constant temperatureit follows an almost linear relationship with pressure.

The variation of the thermal expansion coefficient with thepressures and temperatures can be seen in Fig. 6. It is clear thatthe temperature dependence of the thermal expansion coefficientsof the three compounds follows a T3 law for low temperature, andgradually increases linearly with the increment of temperatures.The effects of the pressure on the thermal expansion coefficientsare very small at low temperatures; the effects are increasinglyobvious as the temperature increases. As pressure increases, thethermal expansion coefficient decreases rapidly and the effects oftemperature become less and less pronounced, resulting in linearhigh temperature behavior. It is noted that the high temperaturedependence of the thermal expansion coefficient is not linearly atlow pressure, this is an indication of the inadequacy of the quasi-harmonic approximation at high temperatures and low pressures.

Additionally, Fig. 7 illustrates certain systematic trends existingfor the studied group of compounds. There is a linear and mono-tonic decrease of the Debye temperature with increasing the unitcell volume, at various temperatures. Such a trend was also re-ported earlier for the transition metal monocarbides [34]. These re-sults can serve as the first predictions to be checked out by futureworks.

4. Conclusion

In this work, the structural and electronic properties of the Ba2-MgWO6, Ba2NiWO6 and Ba2ZnWO6 compounds were investigatedusing first-principles calculations based on density functional the-ory. The calculated structural parameters obtained are consistentwith the experimental data and other theoretical results. Densityof states and electronic band structure often provide sufficientinformation for a through characterization of the electronic prop-erties of a material. The energy band structure, total and partialdensity of states (DOSs) of the three compounds were calculatedby FP-LAPW method. Our band gaps are in a good agreement withprevious theoretical works and the existing experimental data, thediscrepancy is found less than 10%. Temperature-dependent ther-modynamic properties of Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6,including thermal expansion coefficient, bulk modulus, and heat

capacity, have also been studied in terms of first-principles calcu-lations and quasi-harmonic approach, wherein the thermal elec-tronic and vibrational contributions are considered.

Acknowledgments

This work was supported by the Swiss National Science Founda-tion (NSF) and by the International Relations Office at the Univer-sity of Fribourg.

References

[1] T. Kimura, Y. Tokura, Ann. Rev. Mater. Sci. 30 (2000) 451.[2] F. Litchenberg, A. Herrnberger, K. Weidenman, J. Mannhart, Prog. Solid State

Chem. 29 (2001) 1.[3] S.G. Steward, H.P. Rooksby, Acta Crystallogr. 4 (1951) 503.[4] M.T. Anderson, K.B. Greenwood, G.A. Taylor, Prog. Solid State 22 (1993) 197.[5] D.D. Khalyavin, Jiaping Han, A.M.R. Senos, P.Q. Mantas, J. Mater. Res. 18 (2003)

2600.[6] L. Salgado, F.A. Filho, Mater. Sci. Forum 448 (2008) 591.[7] L.A. Rangel de Aguiar, C.M. Lapa, R.A.F. Sanguinetti, J.A. Aguiar, C.L. da Silva,

D.P.F. Souza, Y.P. Yadava, Mater. Sci. Forum 523 (2005) 498.[8] L.H. Brixner, J. Phys. Chem. 64 (1960) 165.[9] P. Blaha, K. Schwarz, G.K.H. Madsen, D. Kvasnicka, J. Luitz, WIEN2k. An

Augmented Plane Wave Plus Local Orbitals Program for Calculating CrystalProperties, Vienna University of Technology, Vienna, Austria, 2001.

[10] P. Hohenberg, W. Kohn, Phys. Rev. 136 (1964) 86.[11] D.M. Ceperley, B.I. Ader, Phys. Rev. Lett. 45 (1980) 566.[12] J.P. Perdew, S. Burke, M. Ernzerhof, Phys. Rev. Lett. 77 (1996) 3865.[13] P. Dufek, P. Blaha, K. Schwarz, Phys. Rev. B 50 (1994) 7279.[14] E. Engel, S.H. Vosko, Phys. Rev. B 47 (1993) 13164.[15] H.J. Monkhorst, J.D. Park, Phys. Rev. B 13 (1976) 5188.[16] C.N.R. Rao, Perovskites – Encyclopedia of Physical Science and Technology,

third ed., 2003, pp. 707–714.[17] S. Meenakshi, V. Vijayakumar, S.N. Achary, A.K. Tyagi, J. Phys. Chem. Solids 72

(2011) 609.[18] V.S. Filipev, G.E. Shatalova, E.G. Fesenko, Kristallografiya 19 (1974) 386.[19] D.D. Khalyavin, J. Han, A.M.R. Senos, P.Q. Mantas, J. Mater. Res. 18 (2003) 2600.[20] D.E. Cox, G. Shirane, B.C. Fraze, J. Appl. Phys. 38 (1967) 1459.[21] H. Iwakura, H. Einaga, Y. Teraoka, J. Nov. Carbohydr. Res. Sci. 3 (2011) 1.[22] D.D. Khalayavin, J. HangSenos, A.M.R. Senos, P.Q. Mantas, J. Mater. Res. 18

(2003) 2600.[23] M.G. Brik, J. Phys. Chem. Solids 73 (2012) 252.[24] S. Dimitrovska, S. Aleksovska, I. Kuzmanovski, Cent. Eur. J. Chem. 198 (2005)

215.[25] H.W. Eng, P.W. Barnes, B.M. Auer, P.M. Woodward, J. Solid State Chem. 175

(2003) 94.[26] I.N. Belyaev, V.S. Filipev, E.G. Fesenko, Z. Strukt. Khim. 4 (1963) 719.[27] L.J. Sham, M. Schluter, Phys. Rev. Lett. 51 (1983) 1888.[28] H.W. Eng, P.W. Barnes, B.M. Auer, P.M. Woodward, J. Solid State Chem. 175

(2003) 94.[29] B.E. Day et al., J. Solid State Chem. 185 (2012) 107.[30] A. Otero-de-la-Roza, D. Abbasi-Pérez, V. Luaña, Comput. Phys. Commun. 182

(2011) 2232.[31] A. Otero-de-la-Roza, V. Luaña, Comput. Theor. Chem. 975 (2011) 111;

A. Otero-de-la-Roza, V. Luaña, Phys. Rev. B 84 (2011) 024109.[32] J.-P. Poirier, Introduction to the Physics of the Earth’s Interior, Cambridge

University Press, 2000.[33] A.T. Petit, P.L. Dulong, Ann. Chim. Phys. 10 (1819) 395.[34] V. Krasnenko, M.G. Brik, Solid State Sci. 14 (2012) 1431.

Fig. 7. Volume and temperature dependence of Debye temperature of Ba2MgWO6, Ba2NiWO6 and Ba2ZnWO6.

6

http

://do

c.re

ro.c

h